Journal of Non-Crystalline Solids 351 (2005) 2616–2621
Correlation between temperature–pressure dependence
of the a-relaxation and configurational entropy
for a glass-forming polymer
Gustavo Ariel Schwartz a, *, Edurne Tellechea b , Juan Colmenero a,b ,Ángel Alegría b
a Donostia International Physics Center, Paseo Manuel de Lardizabal 4, 20018 San Sebastián, Spain
b Departamento de Física de Materiales UPV/EHU, Unidad de Física de Materiales CSIC-UPV/EHU, Facultad de Química,
Apartado 1072, 20080 San Sebastián, Spain
Available online 26 July 2005
In this work we investigated the temperature–pressure dependence of the relaxation time of the a-relaxation process of poly(vinyl
acetate) (PVAc). By means of dielectric spectroscopy technique the relaxation time of the a-process was measured over a broad
range of frequencies (10 1 –10 7 Hz), pressures (0–300 MPa) and temperatures (320–460 K). Two different approaches were used
to analyze the temperature–pressure dependence of the relaxation time: the phenomenological Vogel–Fulcher–Tammann (VFT)
equation and the pressure extended Adam–Gibbs (PEAG) equation recently proposed. We compared both results and discussed
the validity of the VFT approach for PVAc at different pressures. We found an excellent agreement between the experimental data
and the PEAG equation, which only needs four parameters to describe the complete temperature–pressure dependence of the relaxation
time of the a-process. Finally, we showed that the thermal and volumetric contributions to the configurational entropy are
clearly separated for PVAc.
Ó 2005 Elsevier B.V. All rights reserved.
PACS: 64.70.Pf; 77.22.Gm; 65.60.+a
By cooling at sufficiently high rates many liquids do
not crystallize, becoming supercooled and finally enter
to the glassy state where the molecular motions of the
system are frozen in the time scale of the experiment.
Although the most common way to reach the glassy
state is by decreasing the temperature of the system,
the glass transition can also be approached by applying
high enough pressure to a supercooled liquid. Both
* Corresponding author. Tel.: +34 943 015 389; fax: +34 943 015
E-mail address: email@example.com (G.A. Schwartz).
the increase of pressure and the decrease of temperature
result in slower molecular motions. These two different
ways of approaching the glass transition allow to
separate thermal and volumetric effects and to reach a
better understanding of the glass transition process.
The temperature dependence of the relaxation time of
a supercooled liquid is usually described by the Vogel–
Fulcher–Tammann (VFT) [1–3] empirical equation
given by s(T) =s 0 exp(DT 0 /(T T 0 )). Although the
VFT dependence of the relaxation time with temperature
is, in general, in good agreement with the experimental
data, the lack of any clear physical
interpretation does not help in the understanding of
the nature of the glass transition. However, it has been
shown  that the temperature dependence of the
relaxation time expressed by the VFT equation can be
0022-3093/$ - see front matter Ó 2005 Elsevier B.V. All rights reserved.
G.A. Schwartz et al. / Journal of Non-Crystalline Solids 351 (2005) 2616–2621 2617
derived, under certain assumptions, from the Adam–
Gibbs (AG) theory  which is based on the concept
of the configurational entropy and allows linking the
dynamic and thermodynamic behaviour of the glass
Additionally, the effect of pressure variation on the
dynamics of the a-relaxation process can be very useful
to investigate both thermal and density effects. Some of
the seminal works in this area were done in the sixties
[6–8] and a renewed interest has arisen during the last
years [9–13]. The improvement of the experimental techniques
has made possible to obtain a large amount of
accurate data over broader ranges of pressure, temperature
and frequency and therefore contributes to the better
understanding of the involved processes. Thus, a new
equation describing the behaviour of the structural
relaxation time, s(T,P), as a function of both pressure
and temperature, has been recently proposed . This
equation was derived from the Adam–Gibbs (AG) theory
by writing the configurational entropy, S c , in terms
of the excess of both thermal heat capacity and thermal
In this work the a-relaxation of poly(vinyl acetate)
(PVAc) was studied using dielectric spectroscopy
(10 1 –10 7 Hz) over a temperature range between 320
and 460 K and pressures up to 300 MPa. The temperature–pressure
dependence of the experimental a-relaxation
times was found to be very well described using
an extended AG equation  with thermal and expansion
coefficients determined from calorimetric and PVT
The AG theory, which is based on the assumption of
cooperatively rearranging regions, gives an expression
that relates the relaxation time with the configurational
entropy (S c ) 
s ¼ s 0 exp ; ð1Þ
where C is a material constant and S c is the configurational
entropy. However, since S c is not. accessible
experimentally, it is usually identified with the excess entropy
(S ex = S melt S crystal ). Although there is still an
open debate about this point, some findings seem to suggest
a general validity of the proportionality between S ex
and S c ; under this assumption we identify S c with
S ex and therefore the proportionality constant between
them will only affect the value of C in Eq. (1). Thus S c
can be estimated as 
S c ðT Þ¼ DH melt
Z T melt
DC P ðT 0 Þ
T 0 dT 0 ; ð2aÞ
where DC P ¼ C melt
would be the excess heat
capacity. In many polymers no melt is observed and a
different procedure has to be followed to calculate S c .
Usually C crystal
is identified with C glass
and in order to access
the excess entropy what is calculated is
S c ðT Þ¼
where DC P ¼ C melt
DC P ðT 0 Þ
T 0 dT 0 ; ð2bÞ
and T K is the Kauzmann
temperature, which used to be of the order of T g –
50 K, where the excess entropy would vanish. Generally,
an inverse temperature dependence is assumed for
DC P (DC P = K/T) and therefore, by integrating equation
(2b) and replacing S c in Eq. (1), withT 0 = T K , the VFT
expression for the temperature dependence of the relaxation
time is recovered. However, as we will see in this
work, this temperature dependence for DC P is not always
Recently, Casalini et al.  have proposed an extension
of the Eq. (2) for the configurational entropy (S c )
which also includes pressure as an independent variable
by adding a term related to the pressure change. Thus,
the temperature and pressure dependence of the S c is
DC P ðT 0 Þ
S c ðT ; PÞ ¼g T ðPÞ
T 0 dT 0 g P ðT Þ
dP 0 ;
¼ D oV melt
D oV glass
is the difference of the thermal expansivity of the melt
and the glass; g T and g P are factors which could eventually
depend on pressure and temperature, respectively. If
they are constant then the thermal and volumetric contributions
to the configurational entropy are very well
separated and their relative weights can be estimated.
In addition, if DC P follows a K/T law and g P /g T does
not depend on temperature a VFT behaviour is recovered
at any arbitrary fixed pressure with unique set of
values for s 0 and D. In this case we obtain the pressure
extended AG equation 
sðT ; PÞ ¼s 0 exp
T T ; ð5Þ
T 0 ðPÞ ¼
0 D oV
P 0 dP 0 ; ð6Þ
where s 0 , D and T K are the VFT parameters at atmospheric
pressure, and S 1 is the excess entropy at very
high temperature and atmospheric pressure.
2618 G.A. Schwartz et al. / Journal of Non-Crystalline Solids 351 (2005) 2616–2621
Poly(vinyl acetate) (PVAc) (M w = 93080 g/mol) was
used for this study. The calorimetric glass transition
temperature, T g , was determined by differential scanning
calorimetry (DSC). The inflection point of the C P versus
temperature curve was 34.8 ± 0.1 °C.
3.2. Dielectric measurements under pressure
P = 0.1 MPa
Dielectric measurements were carried out in a pressure
cell (0–300 MPa) supplied by Novocontrol GmbH.
The range 10 1 –10 5 Hz was measured with an EGG5302
lock-in amplifier in combination with a Chelsea dielectric
interface whereas for the range 10 3 –10 7 Hz a
HP4192LF impedance analyzer was used. A full description
of the experimental techniques can be found in reference
. The sample measurements were performed
by frequency sweeps at constant temperature, with stability
better than ±0.1 K, and constant pressure, with
stability better than ±2 MPa.
-1 0 1 2 3 4 5 6 7
T = 391.2K
4. Results and discussion
4.1. Dielectric relaxation spectra and relaxation times
Fig. 1a shows the dielectric loss (e 00 ), as a function of
frequency, under atmospheric pressure, at different temperatures
as determined using the pressure cell. Isothermal
spectra, at various pressures, are shown in Fig. 1b.
The central part of the main peak (i.e. the a-relaxation)
was described using the Alvarez–Alegría–Colmenero
function , which is a particular case of the Havriliak–Negami
ðxÞ e 1 ¼
½1 þðixs HN Þ a Š ;
where De is the relaxation strength, s HN is the relaxation
time and a and b are shape parameters with b ¼
1 0.812ð1 aÞ 0.387 . This last constraint allows reducing
the number of free parameters (without significant
decrease of the fitting quality) and also deducing from
this frequency domain fit the parameters of the corresponding
time domain Kohlrausch–Williams–Watts
(KWW) function .
Fig. 2 shows the Arhenius plot for the relaxation time
of maximal loss s ¼ s max ð¼ s HN ðsinðap=ð2 þ 2bÞÞÞ 1=b
ðsinðabp=ð2 þ 2bÞÞÞ 1=b Þ  at different pressures. Filled
and dashed lines represent the corresponding fits to the
phenomenological and theoretical predictions as explained
below. The experimental data are in very good
agreement with those previously published by OÕReilly
 and by Heinrich and Stoll .
1 2 3 4 5 6 7
Fig. 1. (a) Dielectric loss (e 00 ) at atmospheric pressure and different
temperatures (from left to right: 300.5, 313.5, 326.4, 339.4, 352.3,
365.3, 378.3 and 391.2 [K]). (b) Dielectric loss (e 00 ) at 391.2 K and
different pressures (from left to right: 300, 250, 200, 150, 100, 50 and
4.2. Phenomenological approach
Since the VFT equation has shown to be very useful
for an empirical description of the temperature dependence
of the relaxation times for several glass formers,
it is reasonable to use it as a first approximation. Actually,
some expressions, which are ÔnaturalÕ extensions of
the VFT equation, have been recently proposed [9,
18–20] to describe the temperature–pressure dependence
of the relaxation times. Phenomenological expressions
DðT 0 þ bP þ cP 2 Þ
sðT ; PÞ ¼s 0 exp
T ðT 0 þ bP þ cP 2 Þ
which is a particular case of Eq. (5), were found very
useful to fit the temperature–pressure dependence of
the relaxation time of several glass formers [11,21].
However, by keeping s 0 and D those determined from
atmospheric pressure, it is not possible to describe prop-
G.A. Schwartz et al. / Journal of Non-Crystalline Solids 351 (2005) 2616–2621 2619
erly the experimental data for PVAc by means of Eq. (8)
as shown in Fig. 2 for P = 300 MPa (dashed line). If we
leave s 0 as a free parameter, although the fitting is good,
s 0 varies more than one order of magnitude between
atmospheric pressure and 300 MPa which seems to be
unrealistic to our understanding. A possible explanation
for this atypical behaviour of PVAc could be related
with the strong decrease of DC P with temperature as reported
in the literature  and shown in Fig. 3. As
C P [J/K/mol]
2.2 2.4 2.6 2.8 3.0 3.2
1000/T [K -1 ]
Fig. 2. Relaxation time of the a-process of PVAc as a function of
inverse temperature at different pressures (from top to bottom: 300,
250, 200, 150, 100, 50 MPa, atmospheric pressure (ffi0 MPa)). Dashed
line corresponds to Eq. (8) with P = 300 MPa and s 0 and D those
determined from atmospheric pressure; the experimental data at
P = 0 MPa were fitted with both Eq. (10) and the VFT function (both
curves are overlapped in the figure); filled lines represent the predicted
values (see text) according to Eq. (13) (note that for P = 0 MPa
Eq. (13) reduces to Eq. (10)).
300 320 340 360 380 400 420 440
Fig. 3. Heat capacity (C P ) for both melt and crystal (taken from Ref.
), and excess heat capacity ðDC P ¼ C melt
Þ as a function of
temperature. The dashed line (with non-inverted triangles) represents
the extrapolated values of C crystal
P to temperatures above the glass
transition. The values of DC P (open circles) decrease linearly with
temperature as shown by the linear fit to the data. The thick line
represents the best fit of the DC P data to equation DC P = K/T.
aforementioned, what is generally assumed is that the
temperature dependence of DC P should be not far from
DC P = K/T which yield the VFT equation in the AG
framework. However, as shown in Fig. 3 the PVAc temperature
dependence of DC P is actually much stronger
than the K/T, which means that by using AG the VFT
equation is not recovered. As it was shown above, even
if the VFT is valid to fit the data at any fixed pressure, a
complete temperature–pressure description for the
relaxation time is not possible by using extensions of
the VFT equation like Eq. (8).
Taking all these features into account we have
checked whether the extended Adam–Gibbs frame,
namely Eq. (3) in combination with Eq. (1), can provide
a full description of the temperature–pressure dependence
of the relaxation time.
Heat capacity and thermal effects. Fig. 3 shows the
heat capacity (C P ) and the excess heat capacity (DC P )
for the PVAc in the temperature range of interest. It is
clear from this figure that DC P decreases in a nearly
linear fashion with temperature according to the empirical
equation DC P = b mT, where b = (103.96 ± 0.02)
JK 1 mol
1 and m = (0.21 ± 0.01) JK 2 mol
1 . According
with this, the thermal contribution to the
configurational entropy would be
S c ðT ; P ffi 0Þ ¼g T
DC P ðT 0 Þ
T 0 dT 0
¼ g T ðb lnðT =T K Þ mðT T K ÞÞ. ð9Þ
Thus, by introducing this result in Eq. (1), the temperature
dependence of the relaxation time at atmospheric
pressure would be given by
sðT ; P ffi 0Þ ¼s 0 exp
T ðb lnðT =T K Þ mðT T K ÞÞ
By using Eq. (10) to fit the experimental data we got
log(s 0 [s]) = 14.1 ± 0.1, C/g T = (99041 ± 540) Jmol
and T K = 255.5 ± 0.2 K.
It is interesting to note that even when the VFT equation
is not recovered from the AG theory, it is still valid
as a phenomenological description of the experimental
data. Fig. 2 shows the best fit to the experimental data
(at atmospheric pressure) by using both Eq. (10) and
VFT equation with log(s 0 [s]) = 12.8 ± 0.1, D = 6.6 ±
0.1 and T 0 = 259.8 ± 0.1 K. The difference between both
curves is less than the width of the line and therefore
they are superimposed in the figure.
Thermal expansion and volumetric effects. In order to
calculate the volumetric contribution to the configurational
entropy we need to estimate DðoV =oT Þ P
. The temperature
dependence of the volume was estimated by
plotting the specific volume for PVAc, as given in reference
, versus temperature and taking the slopes
below and above T g . For the different pressures the Tait
2620 G.A. Schwartz et al. / Journal of Non-Crystalline Solids 351 (2005) 2616–2621
∆(δV/δT) [cm 3 K -1 mol -1 ]
0 50 100 150 200 250 300
Fig. 4. D(oV/oT) P as a function of pressure. The data were fitted with
an empirical exponential function (see text).
equation  was used with the parameters reported in
 for the glassy state. Fig. 4 shows the pressure dependence
of DðoV =oT Þ P
so obtained and the best fit to an
empirical exponential decay according to
DðoV =oT Þ P
¼ DðoV =oT Þ P¼0
A½1 expð P=P 0 ÞŠ ð11Þ
with A = (2.15 ± 0.03)10 2 cm 3 K 1 mol
1 , P 0 = (129 ±
5) MPa and D(oV/oT) P =0 = (3.35 ± 0.03)10 2 cm 3 K 1
1 . Therefore the pressure contribution to the configurational
g P DðoV =oT Þ P 0dP 0 P
¼ g P P 0 DðoV =oT Þ P¼0
þ expð P=P 0 Þ 1 .
By using Eqs. (9) and (12) in Eq. (3) and then by
replacing in Eq. (1) we have the following expression
for the temperature–pressure dependence of the relaxation
more significant at high pressures, we estimated an average
value by weighting the data with the corresponding
pressure values. The solid line in Fig. 5 represents this
weighted average for all values. This is an important
result which shows that the temperature and pressure
contributions to the configurational entropy come exclusively
from the respective integrals in Eq. (3).
Once the value of g P /g T is known we can use Eq. (13),
with the parameters previously estimated at atmospheric
pressure (log(s 0 ),C/g T and T K ), to calculate the relaxation
time at any temperature and pressure. Fig. 2 shows
the excellent agreement among experimental data and
the predicted values (filled lines) for the relaxation time
using Eq. (13).
P = 50MPa
P = 100MPa
P = 150MPa
P = 200MPa
P = 250MPa
P = 300MPa
330 360 390 420 450
Fig. 5. Coefficient g P /g T as a function of temperature at different
pressures. Open symbols represent low pressure data whereas full
symbols are used for high pressure data. The line represents the
estimated constant weighted value (see text).
sðT ; PÞ ¼s 0 exp 4 nh
T bln T
T K Þ
A P P 0
þ expð P=P 0 Þ 1
Since we already know the values of log(s 0 ), C/g T and
T K , (determined from the fitting at atmospheric pressure)
we can use the experimental values of the relaxation
time to estimate g P /g T for different temperatures
and pressures. Fig. 5 shows g P /g T values versus temperature
for different pressures; no clear temperature or
pressure dependence is observed besides the experimental
uncertainties. Given that the effect of pressure is
We have shown that even if the phenomenological
VFT equation gives an excellent description of the temperature
dependence of the relaxation time at any given
fixed pressure, the complete description of the temperature–pressure
dependence is not possible by keeping s 0
constant. By leaving s 0 as a free parameter we got an
unreasonable change of s 0 with pressure.
The fit of experimental data with Eq. (13) shows not
only the validity of the AG frame but also that it is a
more general theory which includes the VFT behaviour
G.A. Schwartz et al. / Journal of Non-Crystalline Solids 351 (2005) 2616–2621 2621
as a particular case. It is important to note that in
addition to the thermodynamic data taken from the
literature, only four parameters are needed to fit s
(T, P): log(s 0 ), C/g T and T K (from P = 0 MPa data)
and g P /g T .
The fact that the value of g P /g T is constant is an indication
that thermal and volumetric contributions to the
configurational entropy for PVAc are well separated
and their values are given by the integrals expressions
in Eq. (3).
This work has been supported in part by the Spanish
Ministry of Science and Technology (MICyT) (Project
MAT 2001/0070) and by the Government of the Basque
Country (Project 9/UPV 00206.215-13568/2001).
 H. Vogel, Phys. Z 22 (1921) 645.
 G.S. Fulcher, J. Am. Ceram. Soc. 8 (1923) 339.
 G. Tammann, W. Hesse, Z. Anorg. Allg. Chem. 156 (1926) 245.
 R. Richert, C.A. Angell, J. Chem. Phys. 108 (1998) 9016.
 G. Adam, J.H. Gibbs, J. Chem. Phys. 28 (1965) 139.
 J.M. OÕReilly, J. Polym. Sci. 57 (1962) 429.
 G. Williams, Trans. Faraday Soc. 62 (1966) 1321.
 G. Williams, Trans. Faraday Soc. 62 (1966) 2091.
 S. Corezzi, P.A. Rolla, M. Paluch, J. Ziolo, D. Fioretto, Phys.
Rev. E 60 (1999) 4444.
 R. Casalani, S. Capaccioli, M. Lucchesi, P.A. Rolla, Phys. Rev. E
63 (2001) 031207.
 D. Prevosto, M. Lucchesi, S. Capaccioli, R. Casalini, P.A. Rolla,
Phys. Rev. B 67 (2003) 174202.
 C.M. Roland, R. Casalini, Macromolecules 36 (2003) 1361.
 A. Alegria, D. Gomez, J. Colmenero, Macromolecules 35 (2002)
 C.A. Angell, S. Borick, J. Non-Cryst. Solids 307–310 (2002) 393,
and references therein.
 F. Alvarez, A. Alegria, J. Colmenero, Phys. Rev. B 44 (1991)
A. Hofmann, A. Alegria, J. Colmenero, L. Willner, E. Buscaglia,
N. Hadjichristidis, Macromolecules 29 (1996) 129.
 F. Kremer, A. Scöhnhals, Broadband Sielectric Spectroscopy,
Springer-Verlag, Berlin, 2003, page 64.
 W. Heinrich, B. Stoll, Colloid Polym. Sci. 263 (1985) 873.
 M. Naoki, H. Endou, K. Matsumoto, J. Phys. Chem. 91 (1987)
 C.A. Herbst, R.L. Cook, H.E. King, Nature 361 (1993) 518.
 J.T. Bendler, J.J. Fontanella, M.F. Shlesinger, Phys. Rev. Lett. 87
 D. Gomez Plaza, PhD thesis, Univ. País Vasco, Spain, 2000.
 ATHAS database, http://web.utk.edu/~athas/databank/vinyl/
pvac/pvac.html U. Gaur, B. Wunderlich, J. Phys. Chem. Ref.
Data 10 (1981) 1051;
U. Gaur, B.B. Wunderlich, B. Wunderlich, J. Phys. Chem. Ref.
Data 12 (1983) 29.
 J.E. Mark, Physical Properties of Polymers Handbook, AIP Press,
New York, 1996, Chapter 7.
 J.E. Mc Kinney, R. Simha, Macromolecules 7 (1974) 894.